#------------------------------------------------------------------------------
#$Date: 2026-06-05 01:36:20 +0200 (Fri 05 de Jun de 2026) $
#$Revision: 306224 $
#$URL: svn://www.crystallography.net/cod/cif/7/72/11/7721103.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7721103
loop_
_publ_author_name
'Wessels, Vivien'
'Mikuta, Martina'
'Höppe, Henning A.'
_publ_section_title
;
 Weakly Coordinating Borophosphates -- Ca0.5M(H2O)2[B(PO4)2]•H2O (M
 = Mg, Mn, Co, Zn, Cd)
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D6DT00484A
_journal_year                    2026
_chemical_formula_sum            'B1.5 Ca0.75 H9 O16.5 P3 Zn1.5'
_chemical_formula_weight         510.31
_space_group_crystal_system      trigonal
_space_group_IT_number           152
_space_group_name_Hall           'P 31 2"'
_space_group_name_H-M_alt        'P 31 2 1'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2026-05-08 deposited with the CCDC.	2026-05-28 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   9.4653(2)
_cell_length_b                   9.4653(2)
_cell_length_c                   15.5902(3)
_cell_measurement_reflns_used    40347
_cell_measurement_temperature    300(2)
_cell_measurement_theta_max      29.998
_cell_measurement_theta_min      2.485
_cell_volume                     1209.63(4)
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_diffrn_ambient_temperature      300(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'D8 Venture Bruker'
_diffrn_measurement_method       'generic phi and omega scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0284
_diffrn_reflns_av_unetI/netI     0.0165
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            40265
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.997
_diffrn_reflns_theta_min         2.485
_exptl_absorpt_coefficient_mu    3.816
_exptl_absorpt_correction_T_max  0.7376
_exptl_absorpt_correction_T_min  0.6867
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
 SADABS 2016/2: Krause, L., Herbst-Irmer, R., Sheldrick G.M. & Stalke D.,
 J. Appl. Cryst. 48 (2015) 3-10
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.802
_exptl_crystal_description       block
_exptl_crystal_F_000             1014
_exptl_crystal_size_max          0.083
_exptl_crystal_size_mid          0.075
_exptl_crystal_size_min          0.052
_exptl_transmission_factor_max   0.7376
_exptl_transmission_factor_min   0.6867
_refine_diff_density_max         1.283
_refine_diff_density_min         -0.706
_refine_diff_density_rms         0.095
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.026(15)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.109
_refine_ls_hydrogen_treatment    refxyz
_refine_ls_matrix_type           full
_refine_ls_number_parameters     175
_refine_ls_number_reflns         2354
_refine_ls_number_restraints     12
_refine_ls_restrained_S_all      1.107
_refine_ls_R_factor_all          0.0236
_refine_ls_R_factor_gt           0.0233
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0318P)²+1.6732P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0631
_refine_ls_wR_factor_ref         0.0633
_reflns_Friedel_coverage         0.722
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                2332
_reflns_number_total             2354
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d6dt00484a2.cif
_cod_data_source_block           MM08_c222
_cod_original_cell_volume        1209.63(5)
_cod_original_formula_sum        'B1.50 H9 Ca0.75 O16.50 P3 Zn1.50'
_cod_database_code               7721103
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z+1/3'
'-x+y, -x, z+2/3'
'y, x, -z'
'-x, -x+y, -z+1/3'
'x-y, -y, -z+2/3'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn1 Zn 0.09034(4) 0.54517(5) 0.41666(3) 0.01534(10) Uani 1 1 d . . . . .
Ca1A Ca 0.1141(5) 0.7557(5) 0.2549(2) 0.0282(4) Uani 0.250(2) 1 d . . P . .
Ca1B Ca 0.2443(5) 0.8857(5) 0.2450(2) 0.0282(4) Uani 0.250(2) 1 d . . P . .
P1 P 0.16744(10) 0.38861(10) 0.25378(5) 0.00976(16) Uani 1 1 d . . . . .
P2 P 0.22109(10) 0.38858(10) -0.08714(5) 0.00982(16) Uani 1 1 d . . . . .
O1 O 0.2897(4) 0.8087(4) 0.3807(2) 0.0284(6) Uani 1 1 d D . . . .
H11 H 0.394(3) 0.827(7) 0.357(3) 0.034 Uiso 1 1 d D U . . .
H12 H 0.318(6) 0.867(7) 0.436(2) 0.034 Uiso 1 1 d D U . . .
O2 O 0.2898(4) 0.4815(4) 0.4523(2) 0.0284(6) Uani 1 1 d D . . . .
H21 H 0.399(3) 0.572(4) 0.468(3) 0.034 Uiso 1 1 d D U . . .
H22 H 0.268(6) 0.392(4) 0.493(3) 0.034 Uiso 1 1 d D U . . .
O11 O 0.1823(3) 0.4205(3) 0.15514(14) 0.0117(4) Uani 1 1 d . . . . .
O12 O 0.1394(4) 0.5182(3) 0.29291(16) 0.0190(5) Uani 1 1 d . . . . .
O13 O 0.3130(3) 0.3824(3) 0.28805(16) 0.0171(5) Uani 1 1 d . . . . .
O14 O 0.0182(3) 0.2159(3) 0.26830(16) 0.0123(4) Uani 1 1 d . . . . .
O21 O 0.2385(3) 0.4205(3) 0.01156(14) 0.0116(4) Uani 1 1 d . . . . .
O22 O 0.2161(3) 0.1980(3) 0.10172(16) 0.0121(4) Uani 1 1 d . . . . .
O23 O 0.3789(3) 0.5183(3) -0.12594(16) 0.0194(5) Uani 1 1 d . . . . .
O24 O 0.0694(3) 0.3826(3) -0.12122(16) 0.0169(5) Uani 1 1 d . . . . .
B1 B 0.1538(5) 0.3082(4) 0.0833(2) 0.0098(5) Uani 1 1 d . . . . .
O3 O 0.144(3) 0.011(2) 0.3665(12) 0.050(3) Uiso 0.25 1 d D . P . .
O3B O 0.1351(18) 0.000000 0.333333 0.050(3) Uiso 0.5 2 d S . P . .
H31 H 0.202(16) 0.128(5) 0.350(7) 0.060 Uiso 0.5 1 d D U P . .
H32 H 0.086(14) 0.008(14) 0.420(5) 0.060 Uiso 0.5 1 d D U P . .
O4 O 0.1358(18) 0.1358(18) 0.500000 0.050(3) Uiso 0.5 2 d DS . P . .
O4B O 0.145(3) 0.137(3) 0.4660(12) 0.050(3) Uiso 0.25 1 d . . P . .
H41 H 0.146(18) 0.072(12) 0.452(6) 0.060 Uiso 0.5 1 d D U P . .
H42 H 0.167(17) 0.243(7) 0.473(7) 0.060 Uiso 0.5 1 d D U P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn 0.2839 1.4301 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O12 Zn1 O24 103.51(10) . 5 ?
O12 Zn1 O23 157.17(11) . 3_565 ?
O24 Zn1 O23 91.17(11) 5 3_565 ?
O12 Zn1 O13 91.19(11) . 6_565 ?
O24 Zn1 O13 99.89(11) 5 6_565 ?
O23 Zn1 O13 103.58(11) 3_565 6_565 ?
O12 Zn1 O2 85.83(11) . . ?
O24 Zn1 O2 84.97(12) 5 . ?
O23 Zn1 O2 78.03(11) 3_565 . ?
O13 Zn1 O2 174.80(12) 6_565 . ?
O12 Zn1 O1 77.96(11) . . ?
O24 Zn1 O1 175.02(12) 5 . ?
O23 Zn1 O1 86.04(11) 3_565 . ?
O13 Zn1 O1 84.79(12) 6_565 . ?
O2 Zn1 O1 90.41(11) . . ?
O12 Zn1 Ca1B 127.21(10) . 2_665 ?
O24 Zn1 Ca1B 52.09(10) 5 2_665 ?
O23 Zn1 Ca1B 50.92(11) 3_565 2_665 ?
O13 Zn1 Ca1B 134.08(10) 6_565 2_665 ?
O2 Zn1 Ca1B 50.69(11) . 2_665 ?
O1 Zn1 Ca1B 123.23(11) . 2_665 ?
O12 Zn1 Ca1A 51.01(11) . . ?
O24 Zn1 Ca1A 133.99(10) 5 . ?
O23 Zn1 Ca1A 127.28(11) 3_565 . ?
O13 Zn1 Ca1A 51.99(10) 6_565 . ?
O2 Zn1 Ca1A 123.09(11) . . ?
O1 Zn1 Ca1A 50.54(11) . . ?
Ca1B Zn1 Ca1A 172.88(10) 2_665 . ?
Ca1B Ca1A O4B 86.8(7) . 6_565 ?
Ca1B Ca1A O3 60.6(6) . 6_565 ?
O4B Ca1A O3 55.3(8) 6_565 6_565 ?
Ca1B Ca1A O4 86.4(4) . 3_564 ?
O4B Ca1A O4 11.3(7) 6_565 3_564 ?
O3 Ca1A O4 64.6(7) 6_565 3_564 ?
Ca1B Ca1A O2 79.8(2) . 3_564 ?
O4B Ca1A O2 89.6(6) 6_565 3_564 ?
O3 Ca1A O2 125.8(5) 6_565 3_564 ?
O4 Ca1A O2 78.5(2) 3_564 3_564 ?
Ca1B Ca1A O12 115.8(4) . . ?
O4B Ca1A O12 153.9(7) 6_565 . ?
O3 Ca1A O12 146.4(5) 6_565 . ?
O4 Ca1A O12 147.4(4) 3_564 . ?
O2 Ca1A O12 82.38(16) 3_564 . ?
Ca1B Ca1A O1 70.2(2) . . ?
O4B Ca1A O1 135.7(7) 6_565 . ?
O3 Ca1A O1 80.4(6) 6_565 . ?
O4 Ca1A O1 144.4(4) 3_564 . ?
O2 Ca1A O1 121.1(2) 3_564 . ?
O12 Ca1A O1 68.15(14) . . ?
Ca1B Ca1A O13 134.8(3) . 6_565 ?
O4B Ca1A O13 101.8(6) 6_565 6_565 ?
O3 Ca1A O13 88.0(5) 6_565 6_565 ?
O4 Ca1A O13 109.90(17) 3_564 6_565 ?
O2 Ca1A O13 143.4(2) 3_564 6_565 ?
O12 Ca1A O13 72.14(13) . 6_565 ?
O1 Ca1A O13 73.24(13) . 6_565 ?
Ca1B Ca1A O3B 64.5(4) . 1_565 ?
O4B Ca1A O3B 63.8(7) 6_565 1_565 ?
O3 Ca1A O3B 10.5(5) 6_565 1_565 ?
O4 Ca1A O3B 73.7(4) 3_564 1_565 ?
O2 Ca1A O3B 135.4(2) 3_564 1_565 ?
O12 Ca1A O3B 136.2(2) . 1_565 ?
O1 Ca1A O3B 72.1(3) . 1_565 ?
O13 Ca1A O3B 79.68(19) 6_565 1_565 ?
Ca1B Ca1A O4B 87.1(6) . 3_564 ?
O4B Ca1A O4B 20.7(8) 6_565 3_564 ?
O3 Ca1A O4B 73.1(7) 6_565 3_564 ?
O4 Ca1A O4B 9.5(6) 3_564 3_564 ?
O2 Ca1A O4B 69.3(5) 3_564 3_564 ?
O12 Ca1A O4B 139.9(5) . 3_564 ?
O1 Ca1A O4B 151.4(6) . 3_564 ?
O13 Ca1A O4B 115.7(5) 6_565 3_564 ?
O3B Ca1A O4B 82.6(6) 1_565 3_564 ?
Ca1B Ca1A O2 156.0(3) . 6_565 ?
O4B Ca1A O2 73.3(7) 6_565 6_565 ?
O3 Ca1A O2 114.8(6) 6_565 6_565 ?
O4 Ca1A O2 71.5(3) 3_564 6_565 ?
O2 Ca1A O2 86.57(16) 3_564 6_565 ?
O12 Ca1A O2 81.38(16) . 6_565 ?
O1 Ca1A O2 133.68(18) . 6_565 ?
O13 Ca1A O2 64.42(13) 6_565 6_565 ?
O3B Ca1A O2 115.6(4) 1_565 6_565 ?
O4B Ca1A O2 69.5(5) 3_564 6_565 ?
Ca1B Ca1A O3 67.0(5) . 1_565 ?
O4B Ca1A O3 71.6(8) 6_565 1_565 ?
O3 Ca1A O3 19.0(9) 6_565 1_565 ?
O4 Ca1A O3 81.8(6) 3_564 1_565 ?
O2 Ca1A O3 142.2(5) 3_564 1_565 ?
O12 Ca1A O3 127.7(4) . 1_565 ?
O1 Ca1A O3 64.6(5) . 1_565 ?
O13 Ca1A O3 73.8(4) 6_565 1_565 ?
O3B Ca1A O3 8.6(5) 1_565 1_565 ?
O4B Ca1A O3 90.8(6) 3_564 1_565 ?
O2 Ca1A O3 117.0(5) 6_565 1_565 ?
Ca1B Ca1A H22 85(2) . 3_564 ?
O4B Ca1A H22 74.7(16) 6_565 3_564 ?
O3 Ca1A H22 118.4(18) 6_565 3_564 ?
O4 Ca1A H22 63.4(15) 3_564 3_564 ?
O2 Ca1A H22 16.2(16) 3_564 3_564 ?
O12 Ca1A H22 93.4(16) . 3_564 ?
O1 Ca1A H22 136.9(18) . 3_564 ?
O13 Ca1A H22 140(2) 6_565 3_564 ?
O3B Ca1A H22 128.8(17) 1_565 3_564 ?
O4B Ca1A H22 54.0(16) 3_564 3_564 ?
O2 Ca1A H22 77(2) 6_565 3_564 ?
O3 Ca1A H22 137.1(18) 1_565 3_564 ?
Ca1B Ca1A H31 82(3) . 6_565 ?
O4B Ca1A H31 63(4) 6_565 6_565 ?
O3 Ca1A H31 24(2) 6_565 6_565 ?
O4 Ca1A H31 74(4) 3_564 6_565 ?
O2 Ca1A H31 148(2) 3_564 6_565 ?
O12 Ca1A H31 129(3) . 6_565 ?
O1 Ca1A H31 76(4) . 6_565 ?
O13 Ca1A H31 64(2) 6_565 6_565 ?
O3B Ca1A H31 17(3) 1_565 6_565 ?
O4B Ca1A H31 84(4) 3_564 6_565 ?
O2 Ca1A H31 101(4) 6_565 6_565 ?
O3 Ca1A H31 17(4) 1_565 6_565 ?
H22 Ca1A H31 137(3) 3_564 6_565 ?
Ca1B Ca1A H41 69(3) . 6_565 ?
O4B Ca1A H41 19.5(18) 6_565 6_565 ?
O3 Ca1A H41 39.8(16) 6_565 6_565 ?
O4 Ca1A H41 25.7(6) 3_564 6_565 ?
O2 Ca1A H41 94(4) 3_564 6_565 ?
O12 Ca1A H41 173.1(7) . 6_565 ?
O1 Ca1A H41 118.7(6) . 6_565 ?
O13 Ca1A H41 108(4) 6_565 6_565 ?
O3B Ca1A H41 49.6(19) 1_565 6_565 ?
O4B Ca1A H41 33.5(13) 3_564 6_565 ?
O2 Ca1A H41 93(2) 6_565 6_565 ?
O3 Ca1A H41 58(2) 1_565 6_565 ?
H22 Ca1A H41 82(3) 3_564 6_565 ?
H31 Ca1A H41 55(5) 6_565 6_565 ?
Ca1B Ca1A H42 79(4) . 3_564 ?
O4B Ca1A H42 36.7(10) 6_565 3_564 ?
O3 Ca1A H42 82(3) 6_565 3_564 ?
O4 Ca1A H42 25.8(4) 3_564 3_564 ?
O2 Ca1A H42 53.1(10) 3_564 3_564 ?
O12 Ca1A H42 131(3) . 3_564 ?
O1 Ca1A H42 149(4) . 3_564 ?
O13 Ca1A H42 132(2) 6_565 3_564 ?
O3B Ca1A H42 93(3) 1_565 3_564 ?
O4B Ca1A H42 17.4(11) 3_564 3_564 ?
O2 Ca1A H42 77(4) 6_565 3_564 ?
O3 Ca1A H42 101(3) 1_565 3_564 ?
H22 Ca1A H42 39(2) 3_564 3_564 ?
H31 Ca1A H42 98(4) 6_565 3_564 ?
H41 Ca1A H42 43(3) 6_565 3_564 ?
Ca1B Ca1A H42 112.1(7) . 6_565 ?
O4B Ca1A H42 26.6(17) 6_565 6_565 ?
O3 Ca1A H42 77(3) 6_565 6_565 ?
O4 Ca1A H42 25.8(4) 3_564 6_565 ?
O2 Ca1A H42 86(3) 3_564 6_565 ?
O12 Ca1A H42 127.6(19) . 6_565 ?
O1 Ca1A H42 152(4) . 6_565 ?
O13 Ca1A H42 89(2) 6_565 6_565 ?
O3B Ca1A H42 84(3) 1_565 6_565 ?
O4B Ca1A H42 27.7(14) 3_564 6_565 ?
O2 Ca1A H42 46.8(13) 6_565 6_565 ?
O3 Ca1A H42 90(3) 1_565 6_565 ?
H22 Ca1A H42 70(4) 3_564 6_565 ?
H31 Ca1A H42 77(5) 6_565 6_565 ?
H41 Ca1A H42 46(2) 6_565 6_565 ?
H42 Ca1A H42 43(4) 3_564 6_565 ?
Ca1A Ca1B O3 85.8(7) . 6_565 ?
Ca1A Ca1B O4B 59.7(6) . 6_565 ?
O3 Ca1B O4B 55.0(8) 6_565 6_565 ?
Ca1A Ca1B O3B 86.2(4) . 1_565 ?
O3 Ca1B O3B 10.9(7) 6_565 1_565 ?
O4B Ca1B O3B 64.4(7) 6_565 1_565 ?
Ca1A Ca1B O1 79.9(2) . . ?
O3 Ca1B O1 89.2(6) 6_565 . ?
O4B Ca1B O1 125.2(5) 6_565 . ?
O3B Ca1B O1 78.5(2) 1_565 . ?
Ca1A Ca1B O23 116.0(4) . 2_665 ?
O3 Ca1B O23 154.4(7) 6_565 2_665 ?
O4B Ca1B O23 146.7(5) 6_565 2_665 ?
O3B Ca1B O23 147.5(4) 1_565 2_665 ?
O1 Ca1B O23 82.31(16) . 2_665 ?
Ca1A Ca1B O2 70.4(2) . 3_564 ?
O3 Ca1B O2 135.4(7) 6_565 3_564 ?
O4B Ca1B O2 80.4(6) 6_565 3_564 ?
O3B Ca1B O2 144.3(4) 1_565 3_564 ?
O1 Ca1B O2 121.2(2) . 3_564 ?
O23 Ca1B O2 68.18(14) 2_665 3_564 ?
Ca1A Ca1B O24 134.8(3) . 4_565 ?
O3 Ca1B O24 102.5(6) 6_565 4_565 ?
O4B Ca1B O24 88.8(5) 6_565 4_565 ?
O3B Ca1B O24 109.88(17) 1_565 4_565 ?
O1 Ca1B O24 143.4(2) . 4_565 ?
O23 Ca1B O24 72.18(13) 2_665 4_565 ?
O2 Ca1B O24 73.13(13) 3_564 4_565 ?
Ca1A Ca1B O4 64.3(4) . 3_564 ?
O3 Ca1B O4 63.7(7) 6_565 3_564 ?
O4B Ca1B O4 10.9(5) 6_565 3_564 ?
O3B Ca1B O4 73.6(4) 1_565 3_564 ?
O1 Ca1B O4 135.4(2) . 3_564 ?
O23 Ca1B O4 136.3(2) 2_665 3_564 ?
O2 Ca1B O4 72.0(3) 3_564 3_564 ?
O24 Ca1B O4 79.75(19) 4_565 3_564 ?
Ca1A Ca1B O3 87.4(5) . 1_565 ?
O3 Ca1B O3 20.0(8) 6_565 1_565 ?
O4B Ca1B O3 72.6(7) 6_565 1_565 ?
O3B Ca1B O3 9.1(6) 1_565 1_565 ?
O1 Ca1B O3 69.8(5) . 1_565 ?
O23 Ca1B O3 140.0(5) 2_665 1_565 ?
O2 Ca1B O3 151.3(5) 3_564 1_565 ?
O24 Ca1B O3 115.1(5) 4_565 1_565 ?
O4 Ca1B O3 82.2(6) 3_564 1_565 ?
Ca1A Ca1B O1 155.8(3) . 6_675 ?
O3 Ca1B O1 74.0(6) 6_565 6_675 ?
O4B Ca1B O1 115.3(6) 6_565 6_675 ?
O3B Ca1B O1 71.4(3) 1_565 6_675 ?
O1 Ca1B O1 86.37(16) . 6_675 ?
O23 Ca1B O1 81.41(16) 2_665 6_675 ?
O2 Ca1B O1 133.72(18) 3_564 6_675 ?
O24 Ca1B O1 64.57(13) 4_565 6_675 ?
O4 Ca1B O1 115.8(4) 3_564 6_675 ?
O3 Ca1B O1 69.1(5) 1_565 6_675 ?
Ca1A Ca1B O4B 67.1(5) . 3_564 ?
O3 Ca1B O4B 72.0(7) 6_565 3_564 ?
O4B Ca1B O4B 19.9(8) 6_565 3_564 ?
O3B Ca1B O4B 82.2(6) 1_565 3_564 ?
O1 Ca1B O4B 142.7(5) . 3_564 ?
O23 Ca1B O4B 127.2(4) 2_665 3_564 ?
O2 Ca1B O4B 64.2(5) 3_564 3_564 ?
O24 Ca1B O4B 73.5(4) 4_565 3_564 ?
O4 Ca1B O4B 9.1(4) 3_564 3_564 ?
O3 Ca1B O4B 90.9(6) 1_565 3_564 ?
O1 Ca1B O4B 117.1(5) 6_675 3_564 ?
Ca1A Ca1B H11 94.9(11) . . ?
O3 Ca1B H11 108.3(9) 6_565 . ?
O4B Ca1B H11 148.0(8) 6_565 . ?
O3B Ca1B H11 97.3(8) 1_565 . ?
O1 Ca1B H11 23.4(5) . . ?
O23 Ca1B H11 59.4(5) 2_665 . ?
O2 Ca1B H11 110.8(10) 3_564 . ?
O24 Ca1B H11 122.9(8) 4_565 . ?
O4 Ca1B H11 157.3(9) 3_564 . ?
O3 Ca1B H11 88.3(9) 1_565 . ?
O1 Ca1B H11 79.3(13) 6_675 . ?
O4B Ca1B H11 162.0(12) 3_564 . ?
Ca1A Ca1B H12 171.1(12) . 6_675 ?
O3 Ca1B H12 85.6(13) 6_565 6_675 ?
O4B Ca1B H12 112.8(13) 6_565 6_675 ?
O3B Ca1B H12 85.9(10) 1_565 6_675 ?
O1 Ca1B H12 102.6(9) . 6_675 ?
O23 Ca1B H12 72.9(12) 2_665 6_675 ?
O2 Ca1B H12 114.4(8) 3_564 6_675 ?
O24 Ca1B H12 45.3(7) 4_565 6_675 ?
O4 Ca1B H12 109.3(12) 3_564 6_675 ?
O3 Ca1B H12 85.5(10) 1_565 6_675 ?
O1 Ca1B H12 19.7(7) 6_675 6_675 ?
O4B Ca1B H12 107.6(12) 3_564 6_675 ?
H11 Ca1B H12 90.3(13) . 6_675 ?
Ca1A Ca1B H22 53.5(12) . 3_564 ?
O3 Ca1B H22 115.6(12) 6_565 3_564 ?
O4B Ca1B H22 61.3(12) 6_565 3_564 ?
O3B Ca1B H22 123.4(10) 1_565 3_564 ?
O1 Ca1B H22 122.3(15) . 3_564 ?
O23 Ca1B H22 89.1(9) 2_665 3_564 ?
O2 Ca1B H22 21.6(9) 3_564 3_564 ?
O24 Ca1B H22 83.9(13) 4_565 3_564 ?
O4 Ca1B H22 54.6(12) 3_564 3_564 ?
O3 Ca1B H22 129.8(10) 1_565 3_564 ?
O1 Ca1B H22 148.4(13) 6_675 3_564 ?
O4B Ca1B H22 48.3(13) 3_564 3_564 ?
H11 Ca1B H22 121.2(18) . 3_564 ?
H12 Ca1B H22 128.9(15) 6_675 3_564 ?
Ca1A Ca1B H31 58.2(18) . 6_565 ?
O3 Ca1B H31 29.9(10) 6_565 6_565 ?
O4B Ca1B H31 54(3) 6_565 6_565 ?
O3B Ca1B H31 28.0(17) 1_565 6_565 ?
O1 Ca1B H31 74(3) . 6_565 ?
O23 Ca1B H31 157(3) 2_665 6_565 ?
O2 Ca1B H31 123(3) 3_564 6_565 ?
O24 Ca1B H31 129(2) 4_565 6_565 ?
O4 Ca1B H31 65(3) 3_564 6_565 ?
O3 Ca1B H31 30(2) 1_565 6_565 ?
O1 Ca1B H31 99(2) 6_675 6_565 ?
O4B Ca1B H31 74(3) 3_564 6_565 ?
H11 Ca1B H31 98(3) . 6_565 ?
H12 Ca1B H31 114(2) 6_675 6_565 ?
H22 Ca1B H31 101(3) 3_564 6_565 ?
Ca1A Ca1B H41 73(3) . 6_565 ?
O3 Ca1B H41 44(3) 6_565 6_565 ?
O4B Ca1B H41 16(2) 6_565 6_565 ?
O3B Ca1B H41 55(3) 1_565 6_565 ?
O1 Ca1B H41 127(4) . 6_565 ?
O23 Ca1B H41 151(4) 2_665 6_565 ?
O2 Ca1B H41 92(2) 3_564 6_565 ?
O24 Ca1B H41 82(4) 4_565 6_565 ?
O4 Ca1B H41 20(2) 3_564 6_565 ?
O3 Ca1B H41 64(3) 1_565 6_565 ?
O1 Ca1B H41 100(2) 6_675 6_565 ?
O4B Ca1B H41 28(3) 3_564 6_565 ?
H11 Ca1B H41 149(4) . 6_565 ?
H12 Ca1B H41 98(3) 6_675 6_565 ?
H22 Ca1B H41 75(2) 3_564 6_565 ?
H31 Ca1B H41 52(5) 6_565 6_565 ?
Ca1A Ca1B H42 67(4) . 3_564 ?
O3 Ca1B H42 86.1(12) 6_565 3_564 ?
O4B Ca1B H42 33.0(11) 6_565 3_564 ?
O3B Ca1B H42 96.3(9) 1_565 3_564 ?
O1 Ca1B H42 147(4) . 3_564 ?
O23 Ca1B H42 113.7(9) 2_665 3_564 ?
O2 Ca1B H42 50.3(15) 3_564 3_564 ?
O24 Ca1B H42 69(3) 4_565 3_564 ?
O4 Ca1B H42 22.8(7) 3_564 3_564 ?
O3 Ca1B H42 105.0(10) 1_565 3_564 ?
O1 Ca1B H42 123(4) 6_675 3_564 ?
O4B Ca1B H42 14.1(11) 3_564 3_564 ?
H11 Ca1B H42 157(4) . 3_564 ?
H12 Ca1B H42 110(4) 6_675 3_564 ?
H22 Ca1B H42 36(3) 3_564 3_564 ?
H31 Ca1B H42 86(4) 6_565 3_564 ?
H41 Ca1B H42 42(3) 6_565 3_564 ?
Ca1A Ca1B H42 43.3(14) . 6_565 ?
O3 Ca1B H42 67(3) 6_565 6_565 ?
O4B Ca1B H42 18(2) 6_565 6_565 ?
O3B Ca1B H42 74(3) 1_565 6_565 ?
O1 Ca1B H42 117.1(15) . 6_565 ?
O23 Ca1B H42 138(3) 2_665 6_565 ?
O2 Ca1B H42 70(3) 3_564 6_565 ?
O24 Ca1B H42 99.3(14) 4_565 6_565 ?
O4 Ca1B H42 21.1(12) 3_564 6_565 ?
O3 Ca1B H42 81(3) 1_565 6_565 ?
O1 Ca1B H42 133(2) 6_675 6_565 ?
O4B Ca1B H42 25.8(14) 3_564 6_565 ?
H11 Ca1B H42 136.8(16) . 6_565 ?
H12 Ca1B H42 129.9(18) 6_675 6_565 ?
H22 Ca1B H42 49(3) 3_564 6_565 ?
H31 Ca1B H42 56(4) 6_565 6_565 ?
H41 Ca1B H42 33(3) 6_565 6_565 ?
H42 Ca1B H42 33(4) 3_564 6_565 ?
O13 P1 O12 115.14(16) . . ?
O13 P1 O14 106.01(15) . . ?
O12 P1 O14 111.11(15) . . ?
O13 P1 O11 111.17(14) . . ?
O12 P1 O11 106.11(14) . . ?
O14 P1 O11 107.10(13) . . ?
O24 P2 O23 115.29(16) . . ?
O24 P2 O22 106.20(15) . 4 ?
O23 P2 O22 111.06(15) . 4 ?
O24 P2 O21 111.20(13) . . ?
O23 P2 O21 105.81(14) . . ?
O22 P2 O21 107.07(13) 4 . ?
Zn1 O1 Ca1B 112.02(16) . . ?
Zn1 O1 Ca1A 82.51(14) . . ?
Ca1B O1 Ca1A 29.87(13) . . ?
Zn1 O1 Ca1B 136.37(15) . 6_675 ?
Ca1B O1 Ca1B 82.21(17) . 6_675 ?
Ca1A O1 Ca1B 100.61(16) . 6_675 ?
Zn1 O1 H11 119(3) . . ?
Ca1B O1 H11 86(3) . . ?
Ca1A O1 H11 105(3) . . ?
Ca1B O1 H11 103(3) 6_675 . ?
Zn1 O1 H12 104(3) . . ?
Ca1B O1 H12 131(4) . . ?
Ca1A O1 H12 141(3) . . ?
Ca1B O1 H12 49(4) 6_675 . ?
H11 O1 H12 105.2(19) . . ?
Zn1 O2 Ca1A 111.92(16) . 2_665 ?
Zn1 O2 Ca1B 82.48(14) . 2_665 ?
Ca1A O2 Ca1B 29.79(13) 2_665 2_665 ?
Zn1 O2 Ca1A 136.44(15) . 6_665 ?
Ca1A O2 Ca1A 81.96(16) 2_665 6_665 ?
Ca1B O2 Ca1A 100.37(16) 2_665 6_665 ?
Zn1 O2 H21 118(3) . . ?
Ca1A O2 H21 93(3) 2_665 . ?
Ca1B O2 H21 112(3) 2_665 . ?
Ca1A O2 H21 101(3) 6_665 . ?
Zn1 O2 H22 122(3) . . ?
Ca1A O2 H22 25(3) 2_665 . ?
Ca1B O2 H22 44(4) 2_665 . ?
Ca1A O2 H22 58(4) 6_665 . ?
H21 O2 H22 105.3(19) . . ?
B1 O11 P1 130.1(2) . . ?
P1 O12 Zn1 129.16(16) . . ?
P1 O12 Ca1A 141.88(16) . . ?
Zn1 O12 Ca1A 88.88(12) . . ?
P1 O13 Zn1 137.56(16) . 6_665 ?
P1 O13 Ca1A 134.29(17) . 6_665 ?
Zn1 O13 Ca1A 87.80(13) 6_665 6_665 ?
B1 O14 P1 129.7(2) 5 . ?
B1 O21 P2 130.0(2) . . ?
B1 O22 P2 130.0(2) . 4 ?
P2 O23 Zn1 128.88(16) . 2_664 ?
P2 O23 Ca1B 142.19(17) . 3_564 ?
Zn1 O23 Ca1B 88.86(12) 2_664 3_564 ?
P2 O24 Zn1 137.77(16) . 5 ?
P2 O24 Ca1B 134.13(17) . 4_455 ?
Zn1 O24 Ca1B 87.74(13) 5 4_455 ?
O14 B1 O22 103.4(2) 5 . ?
O14 B1 O11 113.7(3) 5 . ?
O22 B1 O11 111.9(3) . . ?
O14 B1 O21 112.2(3) 5 . ?
O22 B1 O21 113.3(3) . . ?
O11 B1 O21 102.7(2) . . ?
O3B O3 O3 4(4) . 6 ?
O3B O3 Ca1B 124(4) . 6_665 ?
O3 O3 Ca1B 120.4(12) 6 6_665 ?
O3B O3 Ca1A 119(3) . 6_665 ?
O3 O3 Ca1A 117(2) 6 6_665 ?
Ca1B O3 Ca1A 33.6(4) 6_665 6_665 ?
O3B O3 Ca1B 43(4) . 1_545 ?
O3 O3 Ca1B 39.6(9) 6 1_545 ?
Ca1B O3 Ca1B 91.5(9) 6_665 1_545 ?
Ca1A O3 Ca1B 108.5(9) 6_665 1_545 ?
O3B O3 Ca1A 46(3) . 1_545 ?
O3 O3 Ca1A 44.1(17) 6 1_545 ?
Ca1B O3 Ca1A 109.3(10) 6_665 1_545 ?
Ca1A O3 Ca1A 133.0(10) 6_665 1_545 ?
Ca1B O3 Ca1A 25.6(2) 1_545 1_545 ?
O3B O3 H31 85(8) . . ?
O3 O3 H31 85(8) 6 . ?
Ca1B O3 H31 72(9) 6_665 . ?
Ca1A O3 H31 42(9) 6_665 . ?
Ca1B O3 H31 101(7) 1_545 . ?
Ca1A O3 H31 124(7) 1_545 . ?
O3B O3 H32 142(10) . . ?
O3 O3 H32 146(8) 6 . ?
Ca1B O3 H32 94(8) 6_665 . ?
Ca1A O3 H32 89(7) 6_665 . ?
Ca1B O3 H32 155(7) 1_545 . ?
Ca1A O3 H32 132(7) 1_545 . ?
H31 O3 H32 103.5(19) . . ?
O3B O3 H41 161(7) . . ?
O3 O3 H41 165(6) 6 . ?
Ca1B O3 H41 66(6) 6_665 . ?
Ca1A O3 H41 60(5) 6_665 . ?
Ca1B O3 H41 154(6) 1_545 . ?
Ca1A O3 H41 150(5) 1_545 . ?
H31 O3 H41 84(8) . . ?
H32 O3 H41 30(9) . . ?
O3 O3B O3 172(8) 6 . ?
O3 O3B Ca1B 45(4) 6 1_545 ?
O3 O3B Ca1B 128(4) . 1_545 ?
O3 O3B Ca1B 128(4) 6 6_665 ?
O3 O3B Ca1B 45(4) . 6_665 ?
Ca1B O3B Ca1B 93.2(7) 1_545 6_665 ?
O3 O3B Ca1A 51(3) 6 1_545 ?
O3 O3B Ca1A 125(3) . 1_545 ?
Ca1B O3B Ca1A 29.26(16) 1_545 1_545 ?
Ca1B O3B Ca1A 110.7(6) 6_665 1_545 ?
O3 O3B Ca1A 125(3) 6 6_665 ?
O3 O3B Ca1A 51(3) . 6_665 ?
Ca1B O3B Ca1A 110.7(6) 1_545 6_665 ?
Ca1B O3B Ca1A 29.26(16) 6_665 6_665 ?
Ca1A O3B Ca1A 135.6(8) 1_545 6_665 ?
O3 O3B H31 113(6) 6 . ?
O3 O3B H31 66(6) . . ?
Ca1B O3B H31 122(7) 1_545 . ?
Ca1B O3B H31 56(8) 6_665 . ?
Ca1A O3B H31 151(7) 1_545 . ?
Ca1A O3B H31 27(8) 6_665 . ?
O3 O3B H32 162(7) 6 . ?
O3 O3B H32 25(7) . . ?
Ca1B O3B H32 145(5) 1_545 . ?
Ca1B O3B H32 70(5) 6_665 . ?
Ca1A O3B H32 128(5) 1_545 . ?
Ca1A O3B H32 69(5) 6_665 . ?
H31 O3B H32 75(3) . . ?
O4B O4 O4B 170(8) 4_556 . ?
O4B O4 Ca1A 45(4) 4_556 2_665 ?
O4B O4 Ca1A 126(4) . 2_665 ?
O4B O4 Ca1A 126(4) 4_556 6_665 ?
O4B O4 Ca1A 45(4) . 6_665 ?
Ca1A O4 Ca1A 93.4(7) 2_665 6_665 ?
O4B O4 Ca1B 53(3) 4_556 2_665 ?
O4B O4 Ca1B 122(3) . 2_665 ?
Ca1A O4 Ca1B 29.29(16) 2_665 2_665 ?
Ca1A O4 Ca1B 110.9(6) 6_665 2_665 ?
O4B O4 Ca1B 122(3) 4_556 6_665 ?
O4B O4 Ca1B 53(3) . 6_665 ?
Ca1A O4 Ca1B 110.9(6) 2_665 6_665 ?
Ca1A O4 Ca1B 29.29(16) 6_665 6_665 ?
Ca1B O4 Ca1B 135.8(7) 2_665 6_665 ?
O4B O4 H41 147(8) 4_556 . ?
O4B O4 H41 38(7) . . ?
Ca1A O4 H41 151(8) 2_665 . ?
Ca1A O4 H41 58(8) 6_665 . ?
Ca1B O4 H41 160(8) 2_665 . ?
Ca1B O4 H41 42(9) 6_665 . ?
O4B O4 H42 107(8) 4_556 . ?
O4B O4 H42 66(7) . . ?
Ca1A O4 H42 63(7) 2_665 . ?
Ca1A O4 H42 63(8) 6_665 . ?
Ca1B O4 H42 58(7) 2_665 . ?
Ca1B O4 H42 92(8) 6_665 . ?
H41 O4 H42 103.4(19) . . ?
O4 O4B O4B 5(4) . 4_556 ?
O4 O4B Ca1A 124(4) . 6_665 ?
O4B O4B Ca1A 119.0(13) 4_556 6_665 ?
O4 O4B Ca1B 116(3) . 6_665 ?
O4B O4B Ca1B 114(2) 4_556 6_665 ?
Ca1A O4B Ca1B 33.4(4) 6_665 6_665 ?
O4 O4B Ca1A 45(3) . 2_665 ?
O4B O4B Ca1A 40.2(10) 4_556 2_665 ?
Ca1A O4B Ca1A 92.0(9) 6_665 2_665 ?
Ca1B O4B Ca1A 108.5(9) 6_665 2_665 ?
O4 O4B Ca1B 48(3) . 2_665 ?
O4B O4B Ca1B 46.0(18) 4_556 2_665 ?
Ca1A O4B Ca1B 110.1(10) 6_665 2_665 ?
Ca1B O4B Ca1B 133.2(10) 6_665 2_665 ?
Ca1A O4B Ca1B 25.7(2) 2_665 2_665 ?
O4 O4B H32 123(6) . . ?
O4B O4B H32 128(4) 4_556 . ?
Ca1A O4B H32 95(3) 6_665 . ?
Ca1B O4B H32 74(5) 6_665 . ?
Ca1A O4B H32 168(4) 2_665 . ?
Ca1B O4B H32 153(5) 2_665 . ?
O4 O4B H41 112(10) . . ?
O4B O4B H41 115(10) 4_556 . ?
Ca1A O4B H41 81(10) 6_665 . ?
Ca1B O4B H41 51(10) 6_665 . ?
Ca1A O4B H41 145(10) 2_665 . ?
Ca1B O4B H41 161(10) 2_665 . ?
H32 O4B H41 29(10) . . ?
O4 O4B H42 82(6) . . ?
O4B O4B H42 78(6) 4_556 . ?
Ca1A O4B H42 82(9) 6_665 . ?
Ca1B O4B H42 114(9) 6_665 . ?
Ca1A O4B H42 42(7) 2_665 . ?
Ca1B O4B H42 35(7) 2_665 . ?
H32 O4B H42 149(10) . . ?
H41 O4B H42 163(10) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn1 O12 2.030(2) . ?
Zn1 O24 2.034(3) 5 ?
Zn1 O23 2.035(2) 3_565 ?
Zn1 O13 2.036(3) 6_565 ?
Zn1 O2 2.318(3) . ?
Zn1 O1 2.322(3) . ?
Zn1 Ca1B 3.150(4) 2_665 ?
Zn1 Ca1A 3.151(4) . ?
Ca1A Ca1B 1.241(5) . ?
Ca1A O4B 1.95(2) 6_565 ?
Ca1A O3 2.24(2) 6_565 ?
Ca1A O4 2.286(12) 3_564 ?
Ca1A O2 2.353(5) 3_564 ?
Ca1A O12 2.450(5) . ?
Ca1A O1 2.454(5) . ?
Ca1A O13 2.484(4) 6_565 ?
Ca1A O3B 2.534(8) 1_565 ?
Ca1A O4B 2.63(2) 3_564 ?
Ca1A O2 2.706(5) 6_565 ?
Ca1A O3 2.87(2) 1_565 ?
Ca1A H22 1.52(4) 3_564 ?
Ca1A H31 1.64(13) 6_565 ?
Ca1A H41 1.96(13) 6_565 ?
Ca1A H42 2.04(12) 3_564 ?
Ca1A H42 2.04(14) 6_565 ?
Ca1B O3 1.96(2) 6_565 ?
Ca1B O4B 2.25(2) 6_565 ?
Ca1B O3B 2.292(13) 1_565 ?
Ca1B O1 2.345(5) . ?
Ca1B O23 2.446(5) 2_665 ?
Ca1B O2 2.458(5) 3_564 ?
Ca1B O24 2.487(4) 4_565 ?
Ca1B O4 2.532(8) 3_564 ?
Ca1B O3 2.65(2) 1_565 ?
Ca1B O1 2.704(5) 6_675 ?
Ca1B O4B 2.86(2) 3_564 ?
Ca1B H11 2.48(5) . ?
Ca1B H12 2.19(6) 6_675 ?
Ca1B H22 1.88(6) 3_564 ?
Ca1B H31 1.91(15) 6_565 ?
Ca1B H41 1.91(13) 6_565 ?
Ca1B H42 2.17(12) 3_564 ?
Ca1B H42 2.76(13) 6_565 ?
P1 O13 1.506(3) . ?
P1 O12 1.507(3) . ?
P1 O14 1.552(2) . ?
P1 O11 1.560(2) . ?
P2 O24 1.505(3) . ?
P2 O23 1.507(3) . ?
P2 O22 1.552(2) 4 ?
P2 O21 1.561(2) . ?
O1 H11 0.987(14) . ?
O1 H12 0.982(13) . ?
O2 H21 0.985(14) . ?
O2 H22 0.989(13) . ?
O11 B1 1.473(4) . ?
O14 B1 1.457(4) 5 ?
O21 B1 1.474(4) . ?
O22 B1 1.460(4) . ?
O3 O3B 0.525(19) . ?
O3 O3 1.05(4) 6 ?
O3 H31 0.997(14) . ?
O3 H32 0.992(14) . ?
O3 H41 1.45(5) . ?
O3B H31 1.08(7) . ?
O3B H32 1.44(4) . ?
O4 O4B 0.535(19) 4_556 ?
O4 O4B 0.535(19) . ?
O4 H41 0.997(14) . ?
O4 H42 0.995(14) . ?
O4B O4B 1.07(4) 4_556 ?
O4B H32 1.28(11) . ?
O4B H41 0.66(6) . ?
O4B H42 0.92(6) . ?
loop_
_geom_hbond_atom_site_label_D
_geom_hbond_atom_site_label_H
_geom_hbond_atom_site_label_A
_geom_hbond_distance_DH
_geom_hbond_distance_HA
_geom_hbond_distance_DA
_geom_hbond_angle_DHA
_geom_hbond_site_symmetry_A
_geom_hbond_publ_flag
O1 H12 O24 0.982(13) 1.822(17) 2.779(4) 164(4) 3_565 yes
O2 H21 O11 0.985(14) 1.787(16) 2.758(4) 168(5) 2_665 yes
O2 H21 O12 0.985(14) 2.56(4) 3.164(4) 119(3) 2_665 yes
O2 H22 O4 0.989(13) 2.10(4) 2.935(14) 140(4) . yes
O2 H22 O4B 0.989(13) 2.13(5) 2.84(2) 127(4) . yes
O2 H22 O4B 0.989(13) 2.13(3) 3.04(2) 153(4) 4_556 yes
O3 H31 O13 0.997(14) 2.30(3) 3.29(2) 169(11) . yes
O3 H31 O14 0.997(14) 2.61(14) 3.14(2) 113(10) . yes
O3B H31 O13 1.08(7) 2.30(3) 3.215(3) 141(9) . yes
O3 H32 O4 0.992(14) 1.64(10) 2.42(2) 132(10) . yes
O3 H32 O4B 0.992(14) 1.28(11) 1.96(3) 118(9) . yes
O3 H32 O4B 0.992(14) 2.11(9) 2.92(3) 138(10) 4_556 yes
O3B H32 O4 1.44(4) 1.64(10) 2.898(5) 140(7) . yes
O3B H31 O4B 1.08(7) 1.90(11) 2.42(2) 105(5) . yes
O3B H32 O4B 1.44(4) 2.11(9) 3.411(19) 147(7) 4_556 yes
O4B H41 O14 0.66(6) 3.14(14) 3.46(3) 114(16) 6 yes
O4B H41 O3 0.66(6) 1.45(5) 1.96(3) 132(15) . yes
O4B H41 O3 0.66(6) 2.48(7) 2.92(3) 126(13) 6 yes
O4B H41 O3B 0.66(6) 1.96(6) 2.42(2) 128(14) . yes
O3 H32 O4 0.992(14) 1.64(10) 2.42(2) 132(10) . yes
O3 H32 O4B 0.992(14) 1.28(11) 1.96(3) 118(9) . yes
O3 H32 O4B 0.992(14) 2.11(9) 2.92(3) 138(10) 4_556 yes
O4 H41 O3 0.997(14) 1.45(5) 2.42(2) 161(13) . yes
O4 H41 O3 0.997(14) 2.48(7) 3.41(2) 155(11) 6 yes
O4 H41 O3B 0.997(14) 1.96(6) 2.898(5) 156(12) . yes
O4B H41 O3 0.66(6) 1.45(5) 1.96(3) 132(15) . yes
O4B H41 O3 0.66(6) 2.48(7) 2.92(3) 126(13) 6 yes
O4B H41 O3B 0.66(6) 1.96(6) 2.42(2) 128(14) . yes
O4 H42 O2 0.995(14) 1.98(5) 2.935(14) 159(12) . yes
O4 H42 O24 0.995(14) 2.65(13) 3.218(3) 116(10) 5 yes
O4B H42 O2 0.92(6) 1.98(5) 2.84(2) 155(12) . yes
O4B H42 O24 0.92(6) 2.65(13) 3.21(2) 120(11) 5 yes
